Journal of Chemistry
Volume 2018 (2018), Article ID 2093654, 10 pages
https://doi.org/10.1155/2018/2093654

Research Article

Optimization of Preparation Conditions of Novel Adsorbent from Sugar Scum Using Response Surface Methodology for Removal of Methylene Blue

Y. El maguana,¹ N. Elhadiri,¹ M. Bouchdoug,¹ M. Benchanaa,¹ and A. Boussetta²

¹Laboratoire de Recherche sur la Réactivité des Matériaux et l’Optimisation des Procédés «REMATOP», Department of Chemistry, Faculty of Science Semlalia, Cadi Ayyad University, B.P. 2390, Marrakech 40000, Morocco
²Centre de recherche REMINEX, Marrakech, Morocco

Correspondence should be addressed to Y. El maguana; youssefelmaguana@gmail.com

Received 18 January 2018; Accepted 5 March 2018; Published 24 April 2018

Academic Editor: Sabrina Copelli

Copyright © 2018 Y. El maguana et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.

Abstract.

A novel and inexpensive adsorbent was prepared from sugar scum for the removal of methylene blue as an organic pollutant from aqueous solutions. The response surface methodology was used to study the effects of the calcination temperature and time on the yield and the methylene blue adsorption. In order to determine the optimal conditions of the preparation, the Doehlert design and desirability function were applied. The increase in calcination temperature increases the methylene blue adsorption and induces a reduction in yield. The optimal conditions have been identified to be a calcination temperature of 986°C and calcination time of 61 min. The characteristics of the obtained adsorbent were determined using SEM/EDX, and surface functions were obtained based on FTIR and pHpzc. The produced adsorbent had a porous structure and a pHpzc of 12.5. The results showed that the yield was 49.74% and the adsorption of methylene blue was 24.52 mg·g⁻¹ with a contact time of 10 h determined by kinetic test. The sugar scum was found to be an effective material for the preparation of appropriate adsorbent for dye removal from wastewater.

1. Introduction

Industrial liquid effluents containing synthetic organic chemicals are potential sources of pollution. They contaminate all the constituents of the environment: soil, water, and air. The majority of these compounds are toxic or carcinogenic and harmful to organisms even in low concentrations [1]. Among these products, the dyes used in several sectors such as textiles, cosmetics, plastics, pigments units, leather, and paper industries have been considered as the primary pollutant due to their stability and low biodegradability [2].

The complex aromatic structures of the dyes render their degradation difficult in the presence of heat, light, microbes, and oxidizing agents [3]. Thus, the discharge of the dye-bearing wastewater in the environment has been the focus of much research in recent years. The scientific community has become increasingly concerned about the potential impact of those contaminants by developing effective removal techniques. Various treatment processes have been used to remove the dyes from wastewater such as adsorption [2, 4–6], membrane filtration [7], photocatalytic and electrochemical combined treatments [8], combinations of coagulation/flocculation with microfiltration, ultrafiltration and adsorption on activated carbon [9], biodegradation [10], oxidation [11], and ozonation [12].

The adsorption is an effective method for the elimination of dyes from wastewater, especially if the adsorbent is inexpensive, readily available, and does not require any additional pretreatment step before its application. Some advantages of adsorption process are its relative simplicity, low cost, and possible regeneration of the adsorbent [3, 13].

In recent years, there has been increasing interest in the research of the production of adsorbents from the agricultural byproducts and industrial wastes for dye removal. The utilization of those wastes has a positive impact on reducing solid wastes, the production of low-cost materials with high added value, and environment protection. Thus, adsorbents have been prepared from clay materials [14, 15], zeolites [16, 17], siliceous material [18], marble dust [19], sewage sludge [20], chitosan [21], fly ash [22], and peels [23].

Sugar scum is derived from the sugar-refining process through juice carbonatation. It is separated from the sugary juices using filtration and contains primarily precipitated calcium carbonate as well as minerals and organic materials removed in juice purification [24]. It is disposed of in open fields or sold as compost to farmers to neutralize acidic soils and improve their structures [24, 25]. So, the objective of the present study is to prepare an adsorbent from sugar scum for the removal of organic pollutants from aqueous solution. The response surface methodology and multicriteria optimization with a Doehlert design and desirability function were used to study the influence of the calcination temperature and time on the yield and adsorption of methylene blue and to determine the optimal conditions of the preparation. The adsorbent obtained under these experimental conditions was characterized by different methods to determine morphological features, surface functions, and point of zero charge.

2. Materials and Methods

2.1. Preparation of Adsorbent

The sugar scum used in this study was brought from a discharge of sugar factory located in Sidi Bennour, Morocco. It was dried at 110°C for 24 h and crushed and sieved to obtain particle size less than 200 µm. The sugar scum powder was put in a tubular furnace (Carbolite Ltd., UK) and heated at a rate of 10°C/min, held at different calcination temperatures between 400 and 1000°C during desired time, and allowed to cool to room temperature. The product was ground (granulometry less than 200 µm), weighed to determine the yield of the product, and stored in a tightly closed bottle for later experimental uses. All the chemicals used in this study were of analytical reagent grade.

2.2. Response Surface Methodology

Response surface methodology is a mathematical and statistical technique useful for modeling and analyzing problems or responses affected by different factors. It was used to optimize the calcination temperature and time in the experimental domains described in Table 1. The responses analyzed were the yield and adsorption of methylene blue. They were related to calcination temperature and time by a second-order polynomial model given in the following equation:

where is the response of interest (yield () and adsorption of methylene blue ()); and are the coded variables related to calcination temperature () and calcination time (), respectively; is a constant, represents the weight of calcination temperature, and represents the weight of calcinations time; is the interaction effect between the calcination temperature and time; and and can be regarded as a curve shape parameter.

Table 1: Experimental domain for the Doehlert experimental design.

Factor
Undimensional variable
Experimental domain

: calcination temperature (°C)

400 to 1000

: calcination time (min)

30 to 120

To estimate the coefficients of the model, the Doehlert design was applied using NEMROD software (New Efficient Methodology for Research using Optimal Design). This design permits to represent the responses studied in all experimental domains of these two factors with a minimum number of experiments for later predication of responses in each point of the domain. The Doehlert experimental design and the corresponding experimental conditions are given in Table 2. The experimental domain center was repeated four times in order to validate the experimental error and to test the reproducibility of the responses [26, 27].

Table 2: Doehlert’s experimental design and operating conditions.

Experiment
Design of experiment
Operating condition

Temperature (°C)
Time (min)

1
1.0000
0.0000
1000.00
75

2
−1.0000
0.0000
400.00
75

3
0.5000
0.8660
850.00
114

4
−0.5000
−0.8660
550.00
36

5
0.5000
−0.8660
850.00
36

6
−0.5000
0.8660
550.00
114

7
0.0000
0.0000
700.00
75

8
0.0000
0.0000
700.00
75

9
0.0000
0.0000
700.00
75

10
0.0000
0.0000
700.00
75

2.3. Characterization of Adsorbent

2.3.1. Batch Adsorption Tests from Aqueous Solutions

The adsorption capacity of sugar scum powder and calcined sugar scum powders was determined by performing batch mode adsorption. Methylene blue was used as adsorbate to determine the adsorption capacity of adsorbents and also serves as a model compound for adsorption of organic contaminants from aqueous solution. The effect of various parameters such as adsorbent dose, contact time, initial methylene blue concentration, and pH on the adsorption capacity of methylene blue was studied. A defined amount of adsorbent was added to flasks of 100 cm³ containing 50 cm³ of desired concentration of methylene blue solution. The desired pH of the solution was adjusted using 0.1M of HCl and NaOH with a pH meter. The suspensions were mixed on a shaker at 170 rpm during a given time and separated with centrifuge. The residual concentration of methylene blue was determined by the spectrophotometric method (UV-3100PC Spectrophotometer) at 664 nm.

The amount of adsorption at equilibrium was defined as the amount of adsorbate per gram of adsorbent (in mg·g⁻¹) and was calculated by the following equation:

The percentage removal of the methylene blue at equilibrium was calculated using the following relationship:

where and (in mg·L⁻¹) are the initial and equilibrium concentrations in aqueous solution, respectively; (L) is the volume of the solution; and (g) is the mass of the adsorbent.

2.3.2. Adsorbent Yield

The yield of the adsorbent is defined as the ratio of the mass of calcined powder to the mass of sugar scum powder. It was calculated based on the following equation:

where (g) is the mass of calcined powder and (g) is the mass of scum powder.

2.3.3. Characterization Techniques

X-ray powder diffraction analysis of sugar scum powder and optimal adsorbent was carried out in Reminex Managem laboratory in Morocco to identify the various phases present in those materials. Scanning electron microscopy coupled with energy dispersive X-ray spectroscopy (SEM/EDX) was used to examine the morphological features of scum powder and optimal adsorbent as well as to determine its elemental composition using TESCAN VEGA3–EDAX instrument with an accelerating voltage of 20 kV.

The sugar scum powder and optimal adsorbent were analyzed with Fourier-transform infrared (FTIR) spectroscopy on a Nicolet 5700 spectrometer in the scanning range of 4000 to 400 cm⁻¹ (64 scans, at a resolution of 4 cm⁻¹) to identify surface functional groups; the sample was mixed with KBr powder, and the mixture was pressed into pellet.

The pH at point of zero charge (pHpzc) corresponds to the pH at which the surface net charge of the adsorbent is zero. In order to determine the pHpzc, 50 mL of 0.01M NaCl, bubbled with nitrogen gas to expel the dissolved CO₂, was taken, and its initial pH was adjusted between 2 and 12 using 0.1M of HCl and NaOH with a pH meter. Then, 10 mg of adsorbent was added to each flask. These flasks were kept for 72 h, and the final pH of the solutions was measured. The pHpzc of adsorbent was identified by the intersection of the curves [28].

3. Results and Discussion

3.1. Optimization of the Preparation Conditions

To obtain an adequate adsorbent, the calcination temperature and time were optimized under the following operating conditions: adsorbent dose of 4 g·L⁻¹, contact time of 24 h, initial methylene blue concentration of 100 mg·g⁻¹, and at pH of solution.

The Doehlert experimental design and experimental results are given in Table 3. In order to interpret the results, the response surfaces were represented in the domains of interest of temperature and time using NEMROD software (isoresponse curves). The estimated values of coefficients for responses yield () and methylene blue adsorption () are given in Table 4.

Table 3: Doehlert’s experimental design and responses: : yield and : MB adsorption.

Experiment
Design of experiment
Operating condition
Experimental response

Temperature (°C)
Time (min)
(%)
(mg/g)

1
1.0000
0.0000
1000.00
75
49.970
21.179

2
−1.0000
0.0000
400.00
75
86.054
5.786

3
0.5000
0.8660
850.00
114
50.608
22.052

4
−0.5000
−0.8660
550.00
36
83.710
3.057

5
0.5000
−0.8660
850.00
36
60.860
23.690

6
−0.5000
0.8660
550.00
114
83.266
2.729

7
0.0000
0.0000
700.00
75
80.608
10.589

8
0.0000
0.0000
700.00
75
80.796
10.153

9
0.0000
0.0000
700.00
75
80.586
11.026

10
0.0000
0.0000
700.00
75
80.726
10.153

Table 4: Estimated values of coefficients for responses and .

Coefficient
Yield,
MB adsorption,

Significance (%)
Significance (%)

80.679
<0.01
10.480
<0.01

−21.279
<0.01
11.790
<0.01

−3.088
<0.01
−0.568
9.9

−12.667
<0.01
3.002
0.275

−10.536
<0.01
2.202
0.752

−5.663
<0.01
−0.756
21.5

Statistically significant at the level <99.99%. Statistically significant at the level 99%.

3.1.1. The Effect of Factors on the Yield

The analysis of the results which are given in Table 3 shows that the yield () varies between 49.97 and 86.054%. Table 4 and Figure 1 show that the calcination temperature () and calcination time () have a negative influence on the yield. The yield is more influenced by calcination temperature () than by calcination time (). At 1000°C, the yield is reduced by 50% due to the decomposition of the carbonates and formation of new phases (CaO as major phase) and CO₂. Thus, in order to have a better yield, it is necessary to operate at a low calcination temperature.

Figure 1: Variation of yield (, %) as a function of calcination temperature and time.

The yield can be described by the model:

3.1.2. The Effect of Factors on the Adsorption of Methylene Blue ()

As shown in Table 3, the methylene blue adsorption on the calcined sugar scum powder varies between 2.73 and 23.69 mg·g⁻¹. Table 4 and Figure 2 show that the calcination temperature is the predominant factor with a positive impact (), and the increase in calcination temperature produces a significant increase in adsorption of methylene blue. The increase in the calcination temperature increases the release of the CO₂, causing an increase in the dimensions of pores and thus resulting in an increase in the adsorption of methylene blue. Thus, to maximize the methylene blue adsorption, it is necessary to operate at a high calcination temperature.

Figure 2: Variation of the methylene blue adsorption capacity (, mg·g⁻¹) as a function of calcination temperature and time.

The adsorption of methylene blue can be described as follows:

3.1.3. Optimization

To determine optimal conditions of both calcination temperature and time for the preparation of adequate adsorbent from sugar scum powder, the responses are optimized simultaneously using the desirability function included in the NEMROD software. It is based on the transformation of all responses obtained from different scales into an identical scale of desirability (individual desirability). The global desirability function , that is taking into account both the requirements on all the responses , is the geometric mean of the individual desirabilities . The desirability is determined by the following equation [27, 29]:

The desirability function varies in the interval [0, 1]; the value 1 corresponds to the maximum satisfaction (desired value), and 0 corresponds to an unacceptable response [30]. The maximum of the function gives the best global compromise for all the responses in the studied domains and corresponds to optimal experimental conditions. All the information and results of the multicriteria optimization are given in Table 5. After the calculation by the NEMROD software, the response surface corresponding to the maximum of the global desirability function , where there are optimal conditions for the preparation of adsorbent with high yield and good quality, is presented as a three-dimensional plot in Figure 3. The optimal point which corresponds to the maximum of the global desirability function is found for a calcination temperature of 986°C and calcination time of 61 min. At these conditions, the predicted values of the responses calculated from the model for the yield and adsorption of methylene blue were 50.68% and 25.01 mg·g⁻¹, respectively. In order to validate the model, three samples of calcined sugar scum powder were prepared under optimal conditions. The characteristics of the optimal adsorbent were 49.74% for the yield and 24.52 mg·g⁻¹ for the adsorption of methylene blue. The difference between the experiment and the predicted values is very lower which confirm the good accuracy of the model.

Table 5: Characteristics of maximum for responses and .

Response
Lower limit
Target value
Weight
(%)
(%)
(%)
Cal. value
Exp. value

 = yield (%)
40
50
1
100.00
100.00
100.00
50.68
49.74

 = MB adsorption (mg·g⁻¹)
15
25
1
100.00
97.49
100.00
25.01
24.52

Desirability

100.00
98.74
100.00

: partial desirability of response , : minimal partial desirability of response , : maximal partial desirability of response , Cal. value: calculated value, and Exp. value: experimental value.

Figure 3: Variation of the function of desirability as a function of calcination temperature and time.

3.2. Study of the Influence of Some Factors on the Methylene Blue Adsorption

3.2.1. Effect of Adsorbent Dose

The effect of adsorbent dose, ranging from 2 to 20 g·L⁻¹, on the adsorption of methylene blue is depicted in Figure 4. The methylene blue removal increases as the amount of the adsorbent increases and reaches a maximum value at 4 g·L⁻¹ and 16 g·L⁻¹ for optimal adsorbent and sugar scum powder, respectively. These observations could be attributed to an increase in the surface area of the adsorbents and hence the number of available adsorption sites for the adsorption of methylene blue [13, 31]. In addition, the methylene blue removal on optimal adsorbent was found to be greater than that for sugar scum powder. The obtained results may suggest that the calcination at high temperature produces a development of the porosity of the obtained material and therefore the number of active sites, requiring slight dose to reach the equilibrium compared to sugar scum powder.

Figure 4: Effect of adsorbent dose on the adsorption of methylene blue onto optimal adsorbent and sugar scum powder (contact time 24 h; [MB] = 100 mg·L⁻¹; T = 25°C).

3.2.2. Effect of Contact Time

Figure 5 represents the variation of the methylene blue adsorption on optimal adsorbent and sugar scum powder as a function of time. The adsorption increased with contact time at the initial stage of adsorption and almost remained constant after some time. The adsorption process of methylene blue was rapid at the beginning of the process due to the availability of active sites on the exterior surfaces. After the saturation of those active sites, methylene blue entered to the pores of the adsorbent with a slower rate to reach equilibrium time [19, 32]. The contact time which corresponds to the equilibrium state is equal to 2 h for sugar scum powder and 10 h for the adsorbent prepared at optimal conditions. The adsorption rate of methylene blue on optimal adsorbent was found to be highly slower than that for sugar scum powder.

Figure 5: Effect of contact time on the adsorption of methylene blue on optimal adsorbent and sugar scum powder (adsorbent dose = 4 g·L⁻¹; [MB] = 100 mg·L⁻¹; T = 25°C).

This difference might be mainly due to the modification of the physicochemical characteristics of optimal adsorbent caused by the calcination process. The methylene blue amount removed by optimal adsorbent was 24.5 mg·g⁻¹, which is higher than the one obtained for sugar scum powder (13.5 mg·g⁻¹).

3.2.3. Effect of Initial MB Concentration

The effect of initial methylene blue concentration on the amount adsorbed on optimal adsorbent and sugar scum powder is shown in Figure 6. The contact time determined by kinetic tests was 2 h and 10 h for sugar scum powder and optimal adsorbent, respectively. It can be seen that the methylene blue adsorption increased as the initial MB concentration increased from 50 to 200 mg·L⁻¹. This could be explained by the fact that as the concentration gradient between the aqueous solution and the solid phase increases, the diffusion rate of MB increases. Furthermore, for the higher initial aqueous concentrations, the contact probability between methylene blue contained in the aqueous phase and the used adsorbent might be more privileged [19, 32]. Similar results were also obtained by Hamed et al. [19], and they studied MB removal from aqueous solutions by marble dust.

Figure 6: Effect of initial methylene blue concentration on the adsorption capacity of optimal adsorbent and sugar scum powder (adsorbent dose = 4 g·L⁻¹; [MB] = 100 mg·L⁻¹; T = 25°C).

3.2.4. Effect of pH

In order to evaluate the effect of pH on the adsorption process, experiments were carried out in the pH range of 3 to 11. Figure 7 illustrates the adsorption of methylene blue on optimal adsorbent and sugar scum powder versus pH. The contact time determined by kinetic tests was 2 h for sugar scum powder and 10 h for optimal adsorbent. It can be observed that for both adsorbent, the increase in pH from 3 to 11 induces a slight increase in the adsorption of methylene blue from 12.16 to 13.68 mg·g⁻¹ for sugar scum powder and from 24.15 to 24.5 mg·g⁻¹ for optimal adsorbent. This can be attributed to an increase in the number of negatively charge sites, which favors the attraction between the positively charged dye and the negatively charged surface of adsorbent. In addition, the optimal adsorbent was a more effective adsorbent compared to sugar scum powder due to its better specific area and porosity.

Figure 7: Effect of pH on the amount of adsorption of methylene blue (adsorbent dose = 4 g·L⁻¹; [MB] = 100 mg·L⁻¹; T = 25°C).

3.3. Characterization of Adsorbent

The XRD patterns of sugar scum powder and adsorbent prepared under optimal conditions are shown in Figure 8. The comparison of the XRD peaks of Figure 8(a) with JCPDS code number 01-086-2339 revealed that the calcite (CaCO₃) is a primary phase in the sugar scum powder [33, 34]. The peaks of Figure 8(b) were matched with JCPDS code number 01-077-2010, 01-084-1265, and 01-079-0612 which indicated the presence of calcium oxide (CaO), calcium hydroxide (Ca(OH)₂), and magnesium oxide (MgO) in the optimal adsorbent. The main peak appeared at 2θ = 37.4 indicating that CaO is the main phase [33, 34]. Therefore, the calcination of scum powder at optimal conditions produced the decomposition of the carbonate into CaO and MgO.

(a)

(b)

Figure 8: XRD patterns of (a) sugar scum powder and (b) optimal adsorbent.

Figure 9 shows SEM micrographs of sugar scum powder and optimal adsorbent. It illustrates that those materials are formed of agglomeration of small particles with irregular shape. At 986°C, spherical particles were obtained due to the decomposition of carbonates and formation of new phases (CaO and MgO) [31]. In addition, the adsorbent prepared at optimum conditions presents higher porosity than sugar scum powder due to the release of carbon dioxide. The results of the elemental analysis using EDX (Table 6) indicate that sugar scum powder is formed by calcite with large amounts of Ca, C, and O. The optimal adsorbent contains higher amounts of Ca and O and less amount of C due to the decomposition of carbonate. Small amounts of other elements (P, Mg, Si, S, and Al) are observed for sugar scum powder and optimal adsorbent.

(a)

(b)

Figure 9: SEM of (a) sugar scum powder and (b) optimal adsorbent.

Table 6: EDX of sugar scum powder and optimal adsorbent.

Element
Sugar scum powder
Optimal adsorbent

Oxygen (%)
45.73
32.87

Calcium (%)
32.99
62.55

Carbon (%)
16.96
1.16

Phosphorus (%)
1.51
0.92

Magnesium (%)
1.33
1.07

Silicon (%)
0.76
0.50

Sulfur (%)
0.43
0.58

Aluminum (%)
0.29
0.36

Figure 10(a) corresponds to the FTIR spectra of sugar scum powder. The band located at around 3424 cm⁻¹ was attributed to O–H stretching vibration of the adsorbed water [35]. The peaks at 713, 874, 1078, 1424, and 2511 cm⁻¹ were assigned to the calcite (CaCO₃) [19, 31, 35]. The low intensity band at 1630 cm⁻¹ was due to the bending vibrations of strongly adsorbed water [35]. The FTIR spectra of adsorbent prepared under optimal conditions are reported in Figure 10(b). According to Zaki and et al. [36], the peaks located at 3864, 3640, 1440, 517, and 470 cm⁻¹ were attributed to CaO. Peaks at around 3450 and 1625 cm⁻¹ corresponded to OH stretching and bending vibrations [37]. The bands located at 1052 and 900 cm⁻¹ may be ascribed to the carbonate [37]. The absence of the absorption peaks at 713 and 874 cm⁻¹ in the spectra of the adsorbent prepared at optimal conditions indicates that CaCO₃ is turned into CaO during calcination.

(a)

(b)

Figure 10: FTIR spectra of (a) sugar scum powder and (b) optimal adsorbent.

The pHpzc values of sugar scum powder and optimal adsorbent are 8.46 and 12.5, respectively (Figure 11). The calcination of scum powder has increased the pHpzc. When the pH is lower than pHpzc, the surface of the adsorbent gets positively charged, and the surface is negatively charged in pH values higher than pHpzc. Those adsorbents can be considered basic.

Figure 11: The pHpzc values of sugar scum powder and optimal adsorbent.

4. Conclusion

The present study shows that the sugar scum is an effective material for the preparation of appropriate adsorbent for dye removal from wastewater. The Doehlert design and desirability function were used to determine the optimal conditions for the preparation of an adsorbent with high yield and good adsorption quality of methylene blue. The increase in calcination temperature increases the adsorption capacity of methylene blue and reduces the yield. The optimal conditions were identified to be a calcination temperature of 986°C and time of 61 min. At these conditions, the experimental responses for the yield and adsorption capacity of methylene blue were 49.74% and 24.52 mg·g⁻¹, respectively, which are in acceptable agreement with the predicted values. The adsorbent prepared at optimum conditions was a more effective adsorbent compared to sugar scum powder due to its better specific area and porosity. These values reflect an interesting adsorbent power of the prepared adsorbent.

Conflicts of Interest

The authors declare that they have no conflicts of interest.

Acknowledgments

The authors are grateful to the Center of Analyses and Characterization (CAC) of University Caddy Ayyad, Morocco. Also, their respectful thanks go to professors of the REMATOP and REMINEX Managem laboratories in Marrakech, Morocco.

References

J. M. Salman, “Preparation of mesoporous activated carbon from branches of pomegranate trees: optimization on removal of methylene blue using response surface methodology,” Journal of Chemistry, vol. 2013, Article ID 489670, 6 pages, 2013.

D. Li, J. Wang, Z. Guo, J. Li, and J. Shuai, “Pectin gels crossliked by Ca²⁺: an efficient material for methylene blue removal,” Journal of Molecular Liquids, vol. 238, pp. 36–42, 2017.

K. S. Bharathi and S. T. Ramesh, “Removal of dyes using agricultural waste as low-cost adsorbents: a review,” Applied Water Science, vol. 3, no. 4, pp. 773–790, 2013.

I. K. Kapdan and F. Kargi, “Simultaneous biodegradation and adsorption of textile dyestuff in an activated sludge unit,” Process Biochemistry, vol. 37, no. 9, pp. 973–981, 2002.

S. Boumchita, A. Lahrichi, Y. Benjelloun, S. Lairini, V. Nenov, and F. Zerrouq, “Removal of cationic dye from aqueous solution by a food waste: potato peel,” Journal of Materials and Environmental Science, vol. 7, pp. 73–84, 2016.

F. Sakr, A. Sennaoui, M. Elouardi, M. Tamimi, and A. Assabbane, “Adsorption study of methylene blue on biomaterial using cactus,” Journal of Materials and Environmental Science, vol. 6, pp. 397–406, 2015.

I. Galambos, J. M. Molina, P. Jaray, G. Vatai, and E. Bekassy-Molnar, “High organic content industrial wastewater treatment by membrane filtration,” Desalination, vol. 162, pp. 117–120, 2004.

M. G. Neelavannan, M. Revathi, and C. A. Basha, “Photocatalytic and electrochemical combined treatment of textile wash water,” Journal of Hazardous Materials, vol. 149, no. 2, pp. 371–378, 2007.

F. Harrelkas, A. Azizi, A. Yaacoubi, A. Benhammou, and M. N. Pons, “Treatment of textile dye effluents using coagulation–flocculation coupled with membrane processes or adsorption on powdered activated carbon,” Desalination, vol. 235, no. 1–3, pp. 330–339, 2009.

N. Daneshvar, A. R. Khataee, M. H. Rasoulifard, and M. Pourhassan, “Biodegradation of dye solution containing Malachite green: optimization of effective parameters using Taguchi method,” Journal of Hazardous Materials, vol. 143, no. 1-2, pp. 214–219, 2007.

P. K. Malik and S. K. Saha, “Oxidation of direct dyes with hydrogen peroxide using ferrous ion as catalyst,” Separation and Purification Technology, vol. 31, no. 3, pp. 241–250, 2003.

S. Lee, K. Lee, W. M. Wan, and Y. Choi, “Comparison of membrane permeability and a fouling mechanism by pre-ozonation followed by membrane filtration and residual ozone in membrane cells,” Desalination, vol. 178, no. 1–3, pp. 287–294, 2005.

S. Elabbas, L. Mandi, F. Berrekhis, M. Noelle, J. Pierre, and N. Ouazzani, “Removal of Cr(III) from chrome tanning wastewater by adsorption using two natural carbonaceous materials: eggshell and powdered marble,” Journal of Environmental Management, vol. 166, pp. 589–595, 2015.

S. Abouarnadasse, “L’élimination du bleu de méthylène par une argile naturelle de Taza en milieu aqueux,” International Journal of Innovative Research in Advanced Engineering, vol. 1, pp. 313–321, 2014.

H. Sadki and K. Z. M. Saidi, “Adsorption of dyes on activated local clay in aqueous solution,” Journal of Materials and Environmental Science, vol. 5, pp. 2060–2065, 2014.

N. Setthaya, P. Chindaprasirt, S. Yin, and K. Pimraksa, “TiO₂-zeolite photocatalysts made of metakaolin and rice husk ash for removal of methylene blue dye,” Powder Technology, vol. 313, pp. 417–426, 2017.

M. Rahmani, M. Kaykhaii, and M. Sasani, “Application of Taguchi L16 design method for comparative study of ability of 3A zeolite in removal of Rhodamine B and Malachite green from environmental water samples,” Spectrochimica Acta Part A: Molecular and Biomolecular Spectroscopy, vol. 188, pp. 164–169, 2018.

J. Yeon Kim, S. Hee Park, and J. S. Yu, “Anchoring of dye molecules into mesoporous siliceous MCM-48,” Optical Materials, vol. 21, no. 1–3, pp. 349–352, 2002.

M. M. Hamed, I. M. Ahmed, and S. S. Metwally, “Adsorptive removal of methylene blue as organic pollutant by marble dust as eco-friendly sorbent,” Journal of Industrial and Engineering Chemistry, vol. 20, no. 4, pp. 2370–2377, 2014.

S. Athalathil, F. Stüber, C. Bengoa, J. Font, A. Fortuny, and A. Fabregat, “Characterization and performance of carbonaceous materials obtained from exhausted sludges for the anaerobic biodecolorization of the azo dye Acid Orange II,” Journal of Hazardous Materials, vol. 267, pp. 21–30, 2014.

A. C. Li, T. Lou, X. Yan, Y. Long, C. Guangpeng Cui, and X. Wang, “Fabrication of pure chitosan nanofibrous membranes as effective absorbent for dye removal,” International Journal of Biological Macromolecules, vol. 106, pp. 768–774, 2017.

A. Aarfane, A. Salhi, M. El Krati, S. Tahiri, and M. Monkade, “Kinetic and thermodynamic study of the adsorption of Red195 and Methylene blue dyes on fly ash and bottom ash in aqueous medium,” Journal of Materials and Environmental Science, vol. 5, pp. 1927–1939, 2014.

S. De Gisi, G. Lofrano, M. Grassi, and M. Notarnicola, “Characteristics and adsorption capacities of low-cost sorbents for wastewater treatment,” Sustainable Materials and Technologies, vol. 9, pp. 10–40, 2016.

M. A. Kamzon, S. Abderafi, and T. Bounahmidi, “Promising bioethanol processes for developing a biorefinery in the Moroccan sugar industry,” International Journal of Hydrogen Energy, vol. 41, no. 45, pp. 20880–20896, 2016.

A. Bhatnagar, K. K. Kesari, and N. Shurpali, “Multidisciplinary approaches to handling wastes in sugar industries,” Water, Air, & Soil Pollution, vol. 227, no. 1, p. 11, 2016.

A. Baçaoui, A. Dahbi, A. Yaacoubi et al., “Experimental design to optimize preparation of activated carbons for use in water treatment,” Environmental Science & Technology, vol. 36, no. 17, pp. 3844–3849, 2002.

K. Ennaciri, A. Baçaoui, and M. Sergent, “Application of fractional factorial and Doehlert designs for optimizing the preparation of activated carbons from Argan shells,” Chemometrics and Intelligent Laboratory Systems, vol. 139, pp. 48–57, 2014.

R. Baccar, M. Sarra, J. Bouzid, M. Feki, and P. Blanquez, “Removal of pharmaceutical compounds by activated carbon prepared from agricultural by-product,” Chemical Engineering Journal, vol. 211-212, pp. 310–317, 2012.

H. Tounsadi, A. Khalidi, M. Abdennouri, and N. Barka, “Activated carbon from Diplotaxis Harra biomass: optimization of preparation conditions and heavy metal removal,” Journal of the Taiwan Institute of Chemical Engineers, vol. 59, pp. 348–358, 2016.

S. Nejjar, H. El Moussami, S. Dahbi, and L. Ezzine, “Optimisation du controle géométrique des tubes cintrés du système de freinage,” in Xth International Conference on Integrated Design and Production (CPI 2015), Tangier, Morocco, December 2015.

D. Mehta, P. Mondal, and S. George, “Utilization of marble waste powder as a novel adsorbent for removal of fluoride ions from aqueous solution, 2016 removal of fluoride ions from aqueous solution,” Journal of Environmental Chemical Engineering, vol. 4, no. 1, pp. 932–942, 2016.

K. Haddad, S. Jellali, S. Jaouadi, M. Benltifa, A. Mlayahb, and A. H. Hamzaoui, “Raw and treated marble wastes reuse as low cost materials for phosphorus removal from aqueous solutions: efficiencies and mechanisms,” Comptes Rendus Chimie, vol. 18, no. 1, pp. 75–87, 2014.

S. Chraibi, H. Moussout, F. Boukhlifi, H. Ahlafi, and M. Alami, “Utilization of calcined eggshell waste as an adsorbent for the removal of phenol from aqueous solution,” Journal of Encapsulation and Adsorption Sciences, vol. 6, no. 4, pp. 132–146, 2016.

P. H. Jai, J. S. Wook, Y. J. Kyu, K. B. Gil, and L. S. Mok, “Removal of heavy metals using waste eggshell,” Journal of Environmental Sciences, vol. 19, no. 12, pp. 1436–1441, 2007.

S. M. Dizaj, F. Lotfipour, M. Barzegar-jalali, M. Zarrintan, and K. Adibkia, “Physicochemical characterization and antimicrobial evaluation of gentamicin-loaded CaCO₃ nanoparticles prepared via microemulsion method,” Journal of Drug Delivery Science and Technology, vol. 35, pp. 16–23, 2016.

M. I. Zaki, H. Knözinger, B. Tesche, and G. A. H. Mekhemer, “Influence of phosphonation and phosphation on surface acid–base and morphological properties of CaO as investigated by in situ FTIR spectroscopy and electron microscopy,” Journal of Colloid and Interface Science, vol. 303, no. 1, pp. 9–17, 2006.

T. R. Fauziah, M. S. Sangi, T. P. Oetami, I. Qoniah, and D. Prasetyoko, “Calcium oxide from limestone as solid base catalyst in transesterification of Reutealis trisperma oil,” Indonesian Journal of Chemistry, vol. 16, no. 2, pp. 208–213, 2016.